SIRIM QAS International Sdn. Bhd.
(Company No.: 199601037981 (410334-X))
No.1, Persiaran Dato' Menteri, P.O.BOX 7035, Section 2,40700 Shah Alam, Selangor Darul Ehsan, Malaysia
Tel: 03-55446667
Fax: 03-55446688
www.sirim-qas.com.my

TEST REPORTREPORT NO : 2022CE2522

PAGE : 1 OF 5

This Test Report refers only to samples submitted by the applicant to SIRIM QAS International Sdn. Bhd. and tested by SIRIM QAS
International Sdn. Bhd. This Test Report shall not be reproduced, except in full and shall not be used for any purpose by any means orforms (including but not limited to advertising purposes) without written approval from the Head of Quality, Occupational Safety and Health& Environment (QOSHE), SIRIM QAS International Sdn. Bhd. Please refer to the last page of this Test Report for Conditions Relating tothe Use of Test Report.

THIS TEST REPORT IS ISSUED IN SECURED PDF SOFTCOPY
Applicant: SHANGHAI ROVAL ZINC RICH PAINT CORPORATION
No. 393, Fenggong RD. Malu,Jiading, Shanghai, 201801, China.

Manufacturer: SHANGHAI ROVAL ZINC RICH PAINT CORPORATIONNo. 393, Fenggong RD. Malu,Jiading, Shanghai, 201801, China.

Product: ROVAL Cold Galvanizing Compound (R96%)

Reference Standard / : ISO 12944-6:1998
Method of Test
Title: Paints and varnishes - Corrosion protection of steel structures byprotective paint systems -Part 6: Laboratory performance test method.
Description of sample : Received six (6) pieces of test panels of ROVAL Cold Galvanizing
Compound (R96%) for testing. The details were described in the next pages.
Date Received of: 12 September 2022
Complete Application
Job No.

: J20223671964

Description of TestResults: The test results for the submitted test samples of ROVAL Cold Galvanizing
Compound (R96%) are described in next pages.

Issued Date: 18 October 2022

Approved Signatory;......................................................
(ABDUL AZIZ BIN HARON)
Senior Testing Executive......................................................
(HAHNAS BINTI MAHBUT)
Head
Chemical, Polymer and Composite Section
Testing Services Department

REPORT NO : 2022CE2522

PAGE : 2 OF 5

This Test Report refers only to samples submitted by the applicant to SIRIM QAS International Sdn. Bhd. and tested by SIRIM QAS
International Sdn. Bhd. This Test Report shall not be reproduced, except in full and shall not be used for any purpose by any means or forms(including but not limited to advertising purposes) without written approval from the Head of Quality, Occupational Safety and Health &Environment (QOSHE), SIRIM QAS International Sdn. Bhd. Please refer to the last page of this Test Report for Conditions Relating to theUse of Test Report.

Test Result
Product: ROVAL Cold Galvanizing Compound (R 96%)

Brand: ROVAL

Type: Liquid & SprayModel: 25kg, 20kg, 10kg, 2.5kg, 1.0kg & Spray 420ml

Test Method:

ISO 12944-6:2018 Paints and varnishes - Corrosion protection ofsteel structures by protective paint systems -Part 6: Laboratory
performance test method.

Test Condition of Neutral Salt Spray (ISO 9227):
Test Duration:

1440 Hours

Corrosivity category as defined in ISO 12944-2
Durability ranges according to ISO 12944-1
Temperature exposure zone
Salt solution used
pH of collected solution

:::::

C5
High
35ºC
5% of NaCl
6.5 – 7.2

Volume of salt collected in ml/h/80 cm2:

1 – 2 ml/hr

No.

Evaluation parameters1Blistering(ISO 4628-2)
RustingISO 4628-3)
Cracking(ISO 4628-4)
Flaking(ISO 4628-5)
Corrosion at scribe after salt
spray test2345

Scribed width
Scribed direction
Note:::

1 mm
X-cut

Requirements
ISO 12944-6
Clause 6.3 Table 4
Blistering 0 (S0)Results

Remarks

0 (S0)

Pass

Rusting Ri 0

Ri 0

Pass

Cracking 0 (S0)

0 (S0)

Pass

Flaking 0 (S0)

0 (S0)

Pass

Maximum 1.5 mm
corrosion at scribe as
average value

0.0 mmPass*The degree of rusting and rusted area is depicted below based on ISO 4628-3 Table 1.
Table 1 – Degree of rusting and rusted area
Degree of rusting
Rusted area, %
Ri 00
Ri 1
0.05
Ri 2
0.5
Ri 31
Ri 48
Ri 5
40 to 50aa

When measuring the rusted area in Figure A.5, it is only about 35 %. If rust is assessed visually using Figure 5,
the impression of rusted area is 40 % to 50 %. One reason might be that partly delaminated rust flakes are notdistinguished from other rusted areas. But this is negligible because Ri 5 normally is outside any specification.

REPORT NO : 2022CE2522

PAGE : 3 OF 5

This Test Report refers only to samples submitted by the applicant to SIRIM QAS International Sdn. Bhd. and tested by SIRIM QAS
International Sdn. Bhd. This Test Report shall not be reproduced, except in full and shall not be used for any purpose by any means or forms(including but not limited to advertising purposes) without written approval from the Head of Quality, Occupational Safety and Health &Environment (QOSHE), SIRIM QAS International Sdn. Bhd. Please refer to the last page of this Test Report for Conditions Relating to theUse of Test Report.

TESTED SAMPLE PHOTO

Unscribed test sample of ROVAL Cold Galvanizing Compound (R96%) after neutral salt spraytest at 1440 Hours

REPORT NO : 2022CE2522

PAGE : 4 OF 5

This Test Report refers only to samples submitted by the applicant to SIRIM QAS International Sdn. Bhd. and tested by SIRIM QAS
International Sdn. Bhd. This Test Report shall not be reproduced, except in full and shall not be used for any purpose by any means or forms(including but not limited to advertising purposes) without written approval from the Head of Quality, Occupational Safety and Health &Environment (QOSHE), SIRIM QAS International Sdn. Bhd. Please refer to the last page of this Test Report for Conditions Relating to theUse of Test Report.

TESTED SAMPLE PHOTO

Scribed test sample of ROVAL Cold Galvanizing Compound (R96%) after neutral salt spraytest at 1440 Hours

REPORT NO : 2022CE2522

PAGE : 5 OF 5

This Test Report refers only to samples submitted by the applicant to SIRIM QAS International Sdn. Bhd. and tested by SIRIM QAS International Sdn.
Bhd. This Test Report shall not be reproduced, except in full and shall not be used for any purpose by any means or forms (including but not limited toadvertising purposes) without written approval from the Head of Quality, Occupational Safety and Health & Environment (QOSHE), SIRIM QAS
International Sdn. Bhd. Please refer to the last page of this Test Report for Conditions Relating to the Use of Test Report.

CONDITIONS RELATING TO THE USE OF SIRIM QAS INTERNATIONAL TEST REPORT
1.

A Test Report will be issued in respect of Testing Services conducted and shall relate only to the sample actually tested. SIRIM QAS International
makes no warranty whatsoever and the Applicant shall not represent in any manner that any duplication or mass production of the Product is sameas the sample actually tested or that SIRIM QAS International has tested any of the duplicated or mass-produced Product. Measurement uncertainty
shall be included in the Test Report when there is no statement of conformity required. When a statement of conformity to a specification or standard
is applied, the Simple Acceptance Rule is used. Unless otherwise stated, the Acceptance Rule with Guard Band is used.

2.

The Test Report shall not be misused, amended, changed, varied or modified in any manner whatsoever by the Applicant or otherwise.

3.

If the Test Report is to be furnished to any third party or to the public, each such Test Report shall be furnished in full, legible and in its entirety.

4.

The Test Report shall not be reproduced and shall not in any event be used for any advertising purposes or whatsoever without written approval fromthe Head of Quality, Occupational Safety and Health & Environment (QOSHE) of SIRIM QAS International of No 1, Persiaran Dato' Menteri, Building
8, Section 2, P.O. Box 7035, 40700 Shah Alam, Selangor Darul Ehsan.

5.

Customer (Applicant/Manufacture/Factory,etc.) is not permitted to use any SIRIM QAS International, SIRIM or other SIRIM's subsidiaries logo or words
on packaging, sample's manual, technical specification, items and products.

6.

Subject to consent and written approval from the Head of Quality, Occupational Safety and Health & Environment (QOSHE) of SIRIM QAS
International, the customer (Applicant/Manufacture/Factory,etc.) may use SIRIM QAS International logo or word on the promotional materials and theApplicant shall only include the phrase, "A sample of this product has been tested by SIRIM QAS International ...(Test Report No) ...(dated) ...(forwhat test) ...(to which standard)" or such similar words which stress that only the sample was actually tested. This phrase shall only be used for thepurpose of product advertisement or product promotion (eg; brochures/flyers/official website). For avoidance of doubt, the statement shall not be
used on the sample, packaging of the sample, items and products.

7.

In the event there is an investigation from a Government Regulatory Agency concerning the Applicant's Test Report, SIRIM QAS International may
disclose the information pertaining to the Test Report for purposes of such investigation.

8.

In the event the Applicant is found in breach of this provision, SIRIM QAS International, SIRIM and/or other SIRIM's subsidiaries without prejudice toany other rights and remedies may take whatever action necessary including but not limited to:a) Informing and placing a notice in the media;b) Obtaining an injunction from Court (cost on a solicitor-client basis to be borne by the Applicant);c) Refusing to accept any further Product for Testing Services from the Applicant or whosoever related to the Applicant, whether subsidiary orotherwise;d) Instructing the Applicant to withdraw and recall the advertisement, statement or document in question and advertise a clarification and apology toSIRIM QAS International, SIRIM and/or other SIRIM's subsidiaries twice in a national publication of SIRIM QAS International's choice at the
Applicant's sole cost; ande) Informing or lodging a report pertaining the Applicant's Test Report with the relevant authorities.

9.

SIRIM QAS International is committed in supporting an environmentally-friendly business practices by reducing paper consumption, therefore we do notissue any hard copy of Test Report to the Applicant. However, additional certified true copy(ies) or softcopy of the Test Report may be issued uponrequest by the Applicant upon payment of the relevant fee. The certified true copy(ies) or softcopy of test report shall only be given for test reportissued not more than three (3) years from the date of issuance.

10. Issuance of Amendment Report due to the following reasons are chargeable to the Applicant :a) Changes in details of the Applicant name and/or address;b) Changes in details of the Manufacturer's name and/or address;c) Changes in details of the Factory location name and/or address;d) Changes in details of the model and/or type designation
11. However, issuance of Supplementary Report due to the following reasons are FOC :a) Misprints and typo errors;b) Missing technical information as agreed in PP1 form;c) Test data not reported;d) Mistake in reporting of test data
12. Corrections to report shall only be allowed if the date of issuance of the original report has not exceeded 6 months and shall be limited to a maximum
3 times, after either case whichever occurs earlier, an Amendment or a Supplementary Report shall not be issued.